Effect of crumb rubber concentration on the physical and ... ?· Effect of crumb rubber concentration…
Post on 07-Jul-2018
Embed Size (px)
International Journal of the Physical Sciences Vol. 6(4), pp. 684-690, 18 February, 2011 Available online at http://www.academicjournals.org/IJPS ISSN 1992 - 1950 2011 Academic Journals Full Length Research Paper
Effect of crumb rubber concentration on the physical and rheological properties of rubberised bitumen
Nuha S. Mashaan*, Asim H. Ali, Mohamed Rehan Karim and Mahrez Abdelaziz
Center for Transportation Research, Department of Civil Engineering, Faculty of Engineering, University of Malaya, 50603 Kuala Lumpur, Malaysia.
Accepted 18 February, 2011
The increase use of crumb rubber in flexible pavements requires the better understanding of its effect on physical and rheological properties of rubberised bitumen binders. The performance properties of rubberised bitumen binder are influenced by the blending conditions and crumb rubber content. The main objective of this research is to investigate the effect of various crumb rubber content on the physical, rheological properties and rutting resistance of rubberised bitumen. Laboratory tests were conducted to evaluate such related properties of bitumen binder with different rubber contents. The tests undertaken comprise the ductility test, elastic recovery test, penetration test and dynamic shear rheometer (DSR) test. The results showed that the addition of crumb rubber has an effect on the physical properties of rubberised bitumen binders, by increasing its elastic recovery and decreasing its penetration and ductility. The rubberised bitumen binder with higher crumb rubber content has an obvious effect on the rheological properties (increase in complex shear modulus G*, storage modulus G, loss modulus G and decrease in phase angle ). The results indicated that the rubber content has the potential to resist rutting deformation that occurs in road pavement as result of increased traffic loading. Key words: Bitumen, crumb rubber, rubberised bitumen, ductility, elastic recovery, penetration, rheology, viscosity, temperature susceptibility, rutting resistance.
INTRODUCTION In recent years, the researches and applications of rubberised bitumen binders in United States have reported many advantages characteristics like improved resistance to rutting due to high viscosity, high softening point and better resilience, improved resistance to surface initiated, reduce fatigue/ reflection cracking, reduce temperature susceptibility, improved durability, lower pavement maintenance costs, and saving in energy and natural resource by using waste products (Liu et al., 2009). *Corresponding author. E-mail: firstname.lastname@example.org. Tel: +603-79675339. Fax: +603-79552182.
According to Ibrahim et al. (2009) Malaysia production of scrap tyres is about 10 million pieces per annum and they are currently being disposed in an environmentally unfriendly manner. A conventional bitumen 80/100 penetration grade is commonly used in Malaysia and it is subjected to the high traffic load and hot weather. Using of crumb rubber in bitumen modification considered as a sustainable technology which transforms an unwanted residue into a new bituminous mixture highly resistant to rutting and fatigue. Since bitumen is viscoelastic material, its rheological properties are very sensitive to temperature as well as rate of loading. The improvement of the properties of rubberised bitumen likely depends on the interaction between crumb rubber and bitumen binder where crumb rubber modifier (CRM) particles swell in the
bitumen binders to form a viscous gel; resulting in an increase in the viscosity of the rubberised bitumen (Airey et al., 2003; Zanzotto and Kennepohl, 1996; Yildirim, 2007; Jeong et al., 2010; Bahia and Davis, 1994). In addition, rheology can be defined as a material property describing mechanical behaviour under various deformation conditions when materials display abilities to flow and recover their original shape after deformation (Widyatmoko and Elliot, 2008). However, the properties of rubberised bitumen binders at a wide range of temperature are largely depending on the chemistry of the bitumen binder, the crumb rubber percentage, particle size, and texture service, blending temperature and blending time. From the previous literature, it was concluded that swelling of the rubber particles due to the absorption of the light fractions oil and stiffening of the residual binder phase are the main mechanism of the interaction (Airey et al., 2003; Abdelrahman and Carpenter, 1999; Shen and Amirkhanian, 2005). Another study by Katman et al. (2005a, 2005b) on using crumb rubber in porous asphalt showed that the blending procedure and mixing type also affect the performance of the rubberized porous asphalt. From an environment and economic standing point, the use of ground tyre rubber as bitumen modifying agent may contribute to solving a waste disposal problem and to improving the quality of road pavement. The main objective of this research study is to investigate the effect of various crumb rubber content on the physical, rheological properties and rutting resistance of rubberised bitumen through selected binder tests. EXPERMMENTAL PROGRAM Materials Bitumen binder grade 80/100 penetration was used in this study. This binder has wide use in different areas especially in Malaysia, the physical properties of this binder given in Table 1. The crumb rubber modifier (CRM) produced by mechanical shredding at ambient temperature was obtained from (Rubberplas Sdn. Bhd.) passing the 30-mesh sieve used with chemical components as shown in Table 2. Preparation of rubberised bitumen binder The rubberised bitumen binder was prepared in the laboratory at blending temperature of 180C (Navarro et al., 2004) and blending time of 60 min (Jeong et al., 2010). Five different concentrations of crumb rubber were prepared by first heating the bitumen to 180C. Upon reaching 180C, a weighted amount of rubber (4, 8, 12, 16 and 20% by weight of bitumen binder) were slowly added to the original bitumen while mixing at 180C using the propeller blade mixer at a blending speed of 200 rpm for blending times of 1 h. Experiments Standard laboratory tests for this research were used, namely, penetration test (ASTM D5), ductility test (ASTM D 113), elastic
Mashaan et al. 685
Table 1. Properties of the base bitumen binder.
Test properties Results Viscosity at 135C (Pa.s) 0.65 G*/ sin at 64C (kPa) 1.35 Ductility at 25C (cm) >100 Softening point (C) 47 Penetration at 25C (d-mm) 88
Table 2. Chemical components of crumb rubber used in the study.
Major rubber components Tire rubber Acetone extract (%) 11.0 Rubber hydrocarbon (%) 50.5 Carbon black content (%) 32.5 Natural rubber content (%) 34.0 Ash content (%) 6.0
recover test (ASTM D 6084) and dynamic shear rheometer (DSR) (ASTM D-4 proposal P246). Penetration, ductility and elastic recovery tests were conducted at temperature of 25C, while the rheological parameters of DSR test were conducted at temperature of 76C and the oscillation chosen is 1.59 Hz (10 rad/s) as this is meant to simulate the shear stress corresponding to traffic speed of 90 km/h (55 mph). RESULTS AND ANALYSIS Ductility test results The ductility test was conducted in accordance with ASTM D113. It provides a measure of tensile properties of bituminous materials. The ductility is measured by the distance in centimetres to which standard specimen will elongate before breaking. The ductility result was conducted at 25C for different crumb rubber contents as illustrated in Figure 1 that shown there is a dramatically decrease in ductility values.
The averages decreased in ductility of modified binder samples compared with unmodified binder were about (18 and 57%) for crumb rubber content of 4 and 20% respectively. In addition, the high amount of crumb rubber in samples 12, 16 and 20% appears to be linear and have constant effect on modified binder under elongation tensile force with correlation coefficient R =0.9991. These results could be explained by the physical interactions during the blending process of the rubberised bitumen.
Accordingly, an increase in binder mass could make the binder more elastic, stiff and highly resistant to pavement rutting. Meanwhile, the decrease in ductility value could be attributed to the oily part of the bitumen
686 Int. J. Phys. Sci.
Crumb rubber content (%)
Figure 1. Ductility test results for different crumb rubber content.
Crumb rubber content (%)
Figure 2. Elastic recovery test results for different crumb rubber content.
absorbed into the rubber powder and the increase in mass of the rubber particles. In effect, the modified binder became thicker compared with the unmodified bitumen samples (Figure 1). Elastic recovery results The elastic recovery method test was conducted in
according to ASTM D 6084 at 25C. Figure 2 shows the effect of different crumb rubber contents on elastic recovery. The increase of crumb rubber content has a significant effect on modified bitumen binder, and it shows a linear increase of elastic recovery value of all samples of rubberised bitumen. Figure 2 illustrate the linear increased in elastic recovery as R = 0.95 which ranges between 21 and 88% for CRM content between 4 and 20% respectively.
Mashaan et al. 687
Crumb rubber content (%)
Figure 3. Penetration test results for different crumb rubber content.
Elastic recovery results were similar to ductility results of rubberised bitumen as it shows significant effect of high content of c